Review Article Volume 4 Issue 4

College of Civil Engineering, Hunan University, China

**Correspondence:** Hyeon-Jong Hwang, College of Civil Engineering, Hunan University, Changsha, Hunan, China, Tel 86 1357 4826 119

Received: August 09, 2018 | Published: August 30, 2018

**Citation: **Hwang HJ. Parametric study on local impact damage of concrete members. *MOJ Civil Eng*. 2018;4(4):369-372. DOI: 10.15406/mojce.2018.04.00130

To predict the local damage of a concrete target subjected to impact load, various empirical and theoretical equations were proposed because the local failure mechanism of concrete on collision is complicated. In the present study, using an empirical model and an energy based model, a parametric study was performed to investigate the effects of design parameters on the penetration depth. All design parameters including concrete strength, rebar ratio, concrete density, aggregate size, steel fiber volume ratio, impact velocity, projectile mass, projectile diameter, and concrete target configuration were considered. The results showed that the energy based model is useful to predict the penetration depth of the local impact-damaged concrete target under various design conditions.

**Keywords: **impact load, penetration, kinetic energy, resistant energy, energy-based penetration model

High-velocity impact causes local failure in reinforced concrete structures.^{1,2} For civilian and military structures under impact load, the impact load resistance needs to be accurately evaluated. However, due to the complicated mechanism of concrete subjected to impact load, the impact resistance of concrete members has been studied by a number of tests and empirical methods. In order to predict the penetration depth of concrete targets, Petry et al.^{2} proposed a method based on a simplified equation of motion for the first time, considering the projectile mass, impact velocity, sectional area of the projectile, and factor related to concrete penetrability. Army Corps of Engineers (ACE)^{3} evaluated the allowable concrete target thickness to restrain significant local failure, and National Defense Research Committee (NDRC)^{4} and Kennedy^{5} additionally considered the nose shape effect of the projectile in ACE model.^{4} The effects of maximum aggregate size, elastic modulus of the projectile, strain-rate of concrete, thickness of the concrete target, concrete density, configuration of the projectile, and hybrid-fibers on the penetration depth of the concrete target have been studied.^{6-15} Unlike empirical models, Hwang et al.^{16} developed an energy-based model for the penetration depth and residual velocity of a projectile. Comparing the kinetic energy of a projectile with the resistant energy of a concrete target directly, the penetration depth of the concrete target can be estimated. Although the energy-based model predicts well the penetration depth of the concrete target, it is difficult to understand the effect of each design parameter on the penetration depth intuitionally in initial design stage. Thus, to investigate the impact damage of the concrete target under high velocity impact, a parametric study was performed. The modified NDRC model^{5} and energy-based model^{16} were used, and the penetration depth of the local impact-damaged concrete target under various design conditions was examined. The analysis results can provide an insight to researchers and practical engineers.

**Modified NDRC**

The modified NDRC method^{5} was developed based on the test results of plain concrete. Although various design conditions cannot be considered, the modified NDRC method has been widely used for simple calculation. The penetration depth *x* of concrete targets is defined as follows.

$x=2d\sqrt{G}$ for $G\le \text{}1$ (1a)

$x=\left(G+1\right)d$ for $G>\text{}1$ (1b)

$G=3.8\times {10}^{-5}\frac{Nm}{d\sqrt{{{f}^{\prime}}_{c}}}{\left(\frac{{V}_{i}}{d}\right)}^{1.8}$ (in kg, MPa, m/s, and m) (1c)

Where *d* is the projectile diameter; *N* is the nose shape factor (= 0.72 for flat nose, 0.84 for hemispherical nose, 1.0 for blunt nose, and 1.13 for sharp nose); *m* is the projectile mass; *f’ _{c}* is the concrete compressive strength; and

**Energy-based penetration model**

In the study of Hwang et al.,^{16} the penetration depth *x* of concrete targets is estimated by comparing the kinetic energy *E _{K}* of projectile with the resistant energy

${E}_{K}=\frac{m}{2}\left({V}_{i}^{2}-{V}_{r}^{2}\right)$ (2)

Where *V _{r}* is the residual velocity of the projectile after perforation (i.e.,

Figure 1 shows local failure mode of concrete targets. Due to deformation of the projectile and concrete target on collision, the kinetic energy *E _{k}* is absorbed by the deformed energy

${E}_{R}={E}_{DP}+{E}_{DC}+{E}_{S}+{E}_{T}+{E}_{C}$ (3a)

${E}_{DP}+{E}_{DC}=\left[\frac{{A}_{p}L}{2{E}_{p}}+\frac{{A}_{p}^{2}{b}^{3}}{24{E}_{cd}{I}_{g}}\right]{\left(\frac{{\rho}_{p}{V}_{i}^{2}}{2}\right)}^{2}$(3b)

$${E}_{S}\left(x\right)=\left({k}_{s}{k}_{bs}\right)\left[\frac{\pi {f}_{td}}{12}+\frac{{A}_{s}{f}_{y}\text{cos}{\theta}_{s}\text{sin}{\theta}_{s}}{3{\left(d+2x\text{tan}{\theta}_{s}\right)}^{2}}\right]\times \left[4{x}_{}^{3}{\text{tan}}^{2}{\theta}_{s}+6d{x}_{}^{2}\text{tan}{\theta}_{s}+3{d}^{2}x\right]$$

$${E}_{S}$$

for$0\le x\le {t}_{s}$(3c)

${E}_{T}\left(x\right)=\frac{4m}{{\rho}_{p}d}\left(2.2\psi \sqrt{{{f}^{\prime}}_{cd}}\right)\left(x-{t}_{s}\right)\ge 0$ for ${t}_{s}\le x\le h-{t}_{c}$(3d)

$${E}_{C}$$

for $h-2{t}_{c}\le x\le h-{t}_{c}$(3e)

Where *A _{p}* is the cross-sectional area of projectile;

In Eqs 3c–3e, the allowable maximum spalling and scabbing depths *t _{s}* and

${t}_{s}={t}_{c}\text{=}{k}_{1}{k}_{2}{k}_{3}{k}_{4}d\le 0.5h$ (4a)

${k}_{1}\text{=}2.1{\left(\frac{h}{d}\right)}^{0.3}-1.75\ge 0$ (4b)

${k}_{2}\text{=}1-0.025{V}_{f}$ (in %) (4c)

${k}_{3}\text{=}5.94-\left(2.1{\rho}_{c}\right)/1000\le 1$(in kg/m^{3}) (4d)

${k}_{4}\text{=}\text{0}{\text{.23s}}_{a}/d+0.77\ge 1$(4e)

where *k*_{1} is the coefficient related to the concrete target thickness; *k*_{2} is the coefficient related to the steel fiber volume ratio; *k*_{3} is the coefficient related to the concrete density ; ${\rho}_{c}$and *k*_{4} is the coefficient related to the maximum size *s _{a}* of coarse aggregates.

In Eqs. 3b–3e, impact force increases the elastic modulus *E _{cd}*, compressive strength

${\stackrel{.}{\epsilon}}_{c}=2\frac{{\epsilon}_{p}}{h}\sqrt{\frac{{E}_{p}}{{\rho}_{p}}}=\frac{{V}_{i}{}^{2}}{h}\sqrt{\frac{{\rho}_{p}}{{E}_{p}}}$(5a)

${E}_{cd}={E}_{cs}{\left(105\stackrel{.}{{\epsilon}_{c}}\right)}^{0.026}$(5b)

${f}_{td}=f{\left(106\stackrel{.}{{\epsilon}_{c}}\right)}^{0.018}$for ${\stackrel{.}{\epsilon}}_{c}<10/s$(5c)

${f}_{td}=0.0062{f}_{t}{\left({10}^{6}\stackrel{.}{{\epsilon}_{c}}\right)}^{1/3}$for ${\stackrel{.}{\epsilon}}_{c}\ge 10/s$(5d)

${f}_{t}=0.3{f}_{c}^{\text{'}}{}^{2/3}{\left(1+\frac{2}{3}\frac{{l}_{f}}{{d}_{f}}{V}_{f}\right)}^{1/3}$for ${{f}^{\prime}}_{c}<50\text{MPa}$(5e)

${f}_{t}=2.12\text{ln}\left[1+0.1\left({{f}^{\prime}}_{c}+8\right)\right]\left(1+\frac{2}{3}\frac{{l}_{f}}{{d}_{f}}{V}_{f}\right)$ for ${{f}^{\prime}}_{c}\ge 50\text{MPa}$ (5f)

${{f}^{\prime}}_{cd}={{f}^{\prime}}_{c}{\left({10}^{5}{\stackrel{.}{\epsilon}}_{c}/3\right)}^{0.014}$for ${\stackrel{.}{\epsilon}}_{c}<30/s$C (5g)

${{f}^{\prime}}_{cd}=0.012{{f}^{\prime}}_{c}{\left({10}^{5}{\stackrel{.}{\epsilon}}_{c}/3\right)}^{1/3}$for ${\stackrel{.}{\epsilon}}_{c}\ge 30/s$ (5h)

Where ${\stackrel{.}{\epsilon}}_{c}$is the strain rate of concrete; ${E}_{cs}$is the elastic modulus of concrete (=$4700\sqrt{{{f}^{\prime}}_{c}}$in MPa) under static load; *f _{t}* is the concrete tensile strength;

Figure 2 shows the relationship between the penetration depth *x* and resistant energy *E _{R}* corresponding to the kinetic energy

To investigate the effects of design parameters on the penetration depth, a parametric study was performed for a concrete target under impact load. A prototype concrete target has the width *b* = 1000 mm; thickness *h* = 300 mm; concrete density ${\rho}_{c}$= 2350 kg/m^{3}; coarse aggregate size $Sa$= 20 mm; steel fiber volume ratio $Vf$= 0%; and effective reinforcing bar area *A _{s}* = 0 mm

Figure 3 compares the penetration predictions of the modified NDRC model^{5} and energy based model^{16} according to the concrete target parameters. As concrete strength increases, the penetration depth decreases (Figure 3). In general, the prediction of the modified NDRC model^{5} is greater than that of the energy based model.^{16} The penetration depth of the energy based model^{16} is significantly increased at the concrete targets using low strength concrete under impact of *V _{i}* = 600 m/s. This is because the tunneling resistance is additionally generated to absorb the kinetic energy in the concrete target using low strength concrete. Reinforcing bars improve the spalling and scabbing resistance, which decreases the penetration depth and damage (Figure 3B). The use of small aggregate size and concrete with large density increase the penetration depth because the impact force of the projectile easily passes through small coarse aggregate in the concrete target (Figure 3C). The use of steel fibers increases the flexural tensile strength of concrete, which decreases the penetration depth (Figure 3D).

Figure 4 compares the penetration predictions of the modified NDRC model^{5} and energy based model^{16} according to the projectile parameters. As the impact velocity increases, the penetration depth increases. Particularly, the prediction of the energy based model^{16} is significantly increased at *V _{i}* = 600 ~ 700 m/s because the tunneling resistance is activated (Figure 4A). Projectile mass increases the kinetic energy, which increases the penetration depth, but the increase ratio is reduced at a certain level (Figure 4B). Thus, although both the impact velocity and projectile mass increases the impact energy, the impact damage of the concrete target is more vulnerable to the high-velocity impact than the heavy-mass impact. Large projectile diameter increases the resisting area of the concrete target, which decreases the penetration depth.

Figure 5 compares the effect of the number of concrete target on the penetration depth. Single concrete target has a thickness of 300 mm, and dual concrete target consists of two concrete targets with a thickness of 150 mm. Under low-velocity impact, the single concrete target exhibits better penetration resistance than that of the dual concrete target. However, the penetration depth of the single concrete target is significantly increased at *V _{i}* = 600~700 m/s due to tunneling failure. In the dual concrete target, perforation failure occurs in the first target at

Figure 6 shows the minimum thickness of concrete target to avoid perforation failure (i.e., *E _{K} *=

To investigate the effects of design parameters on the local impact damage of concrete members, a parametric study was performed by the modified NDRC model and energy-based model, addressing various design conditions of a concrete member and projectile. The parametric study results showed that the use of higher strength concrete, greater reinforcement ratio, larger aggregate size, lower concrete density, and larger steel fiber volume ratio in concrete target design was desirable to decrease the impact damage and penetration depth. The projectile with high-velocity, heavy mass and small diameter increased the penetration depth. Particularly, compared to the single concrete target, dual concrete target system was more efficient to absorb the large impact energy. To avoid perforation failure effectively in concrete targets, high strength fiber-reinforced concrete should be used. This study can be used to guide the direction of future experimental and theoretical studies.

This research was financially supported by National Key Research Program of China (2016YFC0701400) and National Natural Science Foundation of China (Grant No. 51650110500). The authors are grateful to the authorities for their supports.

The author declares there is no conflict of interest.

- Li J, Wu C, Hao H, et al. Blast Resistance of Concrete Slab Reinforced with High Performance Fibre Material.
*Journal of Structural Integrity and Maintenance*. 2016;1(2):51–59. - Kennedy RP. A Review of Procedures for the Analysis and Design of Concrete Structures to Resist Missile Impact Effects.
*Nuclear Engineering and Design.*1976;37(2):183–203. - ACE.
*Fundamentals of Protective Structures. Report AT120 AT1207821*. Army Corps of Engineers, Office of the Chief of Engineers, USA; 1946. - NDRC. Effects of Impact and Explosion.
*Summary Technical Report of Division 2*, V.1, National Defense Research Committee, Washington, DC, USA; 1946. - Kennedy RP.
*Effects of an aircraft crash into a concrete reactor containment building*. Anaheim, CA: Holmes & Narver Inc., USA; 1966. - Whiffen P.
*UK Road Research Laboratory*. Note No. MOS/311, UK; 1943. - Kar AK. Local Effects of Tornado Generated Missiles.
*Journal of the Structural Division*. 1978;104(5):809–816. - Hughes G. Hard Missile Impact on Reinforced Concrete.
*Nuclear Engineering and Design*. 1984;77(1):23–35. - Kojima I. An Experimental Study on Local Behaviour of Reinforced Concrete Slabs to Missile Impact.
*Nuclear Engineering and Design*. 1991;130(2):121–132. - Reid SR, Wen HM.
*Predicting Penetration, Cone Cracking. Scabbing and Perforation of Reinforced Concrete Targets Struck by Flat–Faced Projectiles*. UMIST Report ME/AM/02.01/TE/G/018507/Z, UK; 2001. - Forrestal MJ, Altman BS, Cargile JD, et al. An Empirical Equation for Penetration Depth of Ogive–Nose Projectiles into Concrete Targets.
*International Journal of Impact Engineering*. 1994;15(4):395–405. - Li QM, Chen XW. Dimensionless Formulae for Penetration Depth of Concrete Target Impacted by A Non–Deformable Projectile.
*International Journal of Impact Engineering*. 2003;28(1):93–116. - Guirgis S, Guirguis E. An Energy Approach Study of the Penetration of Concrete by Rigid Missiles.
*Nuclear Engineering and Design*. 2009;4:819–829. - Almusallam TH, Siddiqui N, Iqbal RA, et al. Response of Hybrid–Fiber Reinforced Concrete Slabs to Hard Projectile Impact.
*International Journal of Impact Engineering*. 2013;58:17–30. - Peng Y, Wu H, Fang Q, et al. A Note on the Deep Penetration and Perforation of Hard Projectiles into Thick Targets.
*International Journal of Impact Engineering*. 2015;85:37–44. - Hwang HJ, Kim S, Kang THK. Energy–Based Penetration Model for Local Impact–Damaged Concrete Members.
*ACI Structural Journal*. 2017;114(5):1189–1200. - Fib.
*fib Model Code for Concrete Structures 2010*. Fib, Ernst & Sohn, Germany. 2010:420. - Musmar M. Tensile Strength of Steel Fiber Reinforced Concrete.
*Contemporary Engineering Sciences*. 2013;6(5):225–237.

©2018 Hwang. This is an open access article distributed under the terms of the, which permits unrestricted use, distribution, and build upon your work non-commercially.